Selective Laser Melting of Aluminium Alloys
Nesma T. Aboulkhair*, Nicola M. Everitt, Ian Maskery, Ian Ashcroft, Chris Tuck
Metal additive manufacturing (AM) processes, such as selective laser melting, enable powdered metals to be formed into arbitrary 3D shapes. For aluminium alloys, which are desirable in many high-value applications for their low density and good mechanical performance, selective laser melting is regarded as challenging due to the difficulties in laser melting aluminium powders.
However, a number of studies in recent years have demonstrated successful aluminium processing, and have gone on to explore its potential for use in advanced, AM componentry. In addition to enabling the fabrication of highly complex structures, selective laser melting produces parts with characteristically fine microstructures that yield distinct mechanical properties. Research is rapidly progressing in this field, with promising results opening up a range of possible applications across scientific and industrial sectors. This paper reports on recent developments in this area of research as well as highlighting some key topics that require further attention
Keywords: Al; Metal; Powder Processing; Rapid Solidification, Fatigue.
Introduction to selective laser melting
Many industrial sectors are now benefiting from the possibility of
temperature-controlled build-plate which acts as a heat sink and aids in heat dissipation by lowering the thermal gradient 10, avoiding part curling due to non-uniform thermal expansion 11.
Modern AM dates back to the mid-1980s and expanded during the late 1980s and early 1990s principally as a method for manufacturing prototypes quickly 12, 13. Only recently has AM been considered part of a new industrial revolution 14. A description of the evolution of AM can be found in 15. SLM is gaining wide popularity across industrial and scientific research sectors 13, 16 for applications in the aerospace, automotive, and biomedical fields 17. Components are fabricated from loose powder with comparable physical shape and properties and often even superior to those conventionally-manufactured (CM) 4, 18. Part of the interest in SLM is driven by raising the level of automation in the
Figure 1. Examples of complex structures manufactured using selective laser melting at the Centre for
Additive Manufacturing (CfAM) laboratories at The University of Nottingham: (a) a stainless steel
diamond lattice structure, (b) titanium designer necklace designed by Carrie Dickens, and (c) a jaw
bone made from stainless steel.
In SLM, a thin layer of feedstock powder is deposited by a wiper or roller mechanism. A laser then scans across the powder-bed line-by-line, melting the powder into cylindrical segments 25; referred to as scan tracks (Figure 2a) or melt pools (Figure 2b). Scan tracks are similar to laser welds with the characteristic chevron pattern on top 26. SLM samples are built up through metallurgical bonding of scan tracks overlapping in the horizontal and vertical directions (Figure 2c).
There are numerous useful reviews on metal AM, such as 12, 28. The reader is directed to reference 29 for a generic review on AM processes. A review
and solidification behaviour, as well as the local and bulk mechanical behaviour of the material.
Figure 1: (a) Characteristic chevron pattern on top of an AlSi10Mg single track processed by SLM on
an LM6 as-cast substrate and (b) cross-sectional view (A-A) of a single melt pool showing evidence of
keyhole-mode melting, (c) isometric view for the orthogonal planes of a selectively laser melted cube
from AlSi10Mg showing the overlapping tracks building up the part 27.
The suitability of aluminium alloys for SLM
A great deal of SLM research to date has focussed on the fabrication of steel and titanium components. Paving the way for SLM to become an attractive alternative to subtractive and forming CM requires widening the range of usable materials. Aluminium alloys are characterised by low density (2.7 gm/cm3), high strength 31, adequate hardenability 32, good corrosion resistance 33-35, and excellent
(a) Scan track
weld-ability 32, making them suitable for use in a range of applications 36, such as automotive, defence and aerospace equipment manufacturing, and machinery and tools production 32, 33, 35. The possibility of manufacturing advanced lightweight Al parts using SLM opens up additional application opportunities and promotes the use of difficult-to-machine alloys. Examples of Al alloys examined for
manufacture by SLM are shown in Table I, with AlSi10Mg having so far received the most attention. Further details on the classification of the Al alloys studied for SLM in the literature are available in 37.
Table I: Summary of works done in the field of SLM of Al alloys in the different focus areas
listing the references.
Single tracks &
AlSi10Mg 26, 47 38, 45 43, 48-52 20, 49, 52, 53
Al-2618 54 54
Al-2219 54 54
Al-7075 46 46 46, 55
A357 56 56
AlSi50 57, 58
AlSi12 42, 59 60 42, 60
The challenges of processing aluminium alloys by SLM
absorption of Al is poor 40 suggesting the need for high laser power to overcome the rapid heat dissipation 35. They are highly susceptible to oxidation 8, 33, 41, 42, which promotes porosity 40, 43, 44 alongside their low melt viscosity 40. The major challenges addressed in the literature include minimizing porosity 22, 38, 45 and cracking 46.
Numerous processing parameters are associated with SLM. These are known to affect the quality of the manufactured parts 38, with ‘unoptimised’ parameters introducing defects, mainly porosity 32, 62. The set of optimized parameters varies from one SLM machine to another and between materials. Therefore, “Material Development/Qualification Research” 14, 19 is crucial for the success of the process. The most frequently examined parameters 8 are the
processing environment, powder properties, layer thickness, laser power, scan speed, hatch spacing, and scan strategy 27.
SLM is conducted under inert atmosphere, typically argon 38, 45. Wang et al. 42 reported the type of inert gas to have no effect on densification. However, Ferrar et al. 4 stated that the gas flow rate within the SLM chamber controls the amount of condensate and spatter removed during processing; these ejecta are generated by the laser-material interaction 63, 64, with the amount of spatter related to the laser power and spot size 14. Their structure and chemical composition were shown by Simonelli et al. 64 to be different from the feedstock powder. Inefficient removal of the spatter might lead to its entrapment as inclusions in the final parts, as has been observed by Aboulkhair et al. 53, affecting final part densities.
starting powder significantly suppresses densification 65, 66. Pre-heating the powder is recommended to improve its laser absorptivity 67 and enhance
densification 59. Also, the use of the pre-sinter scan strategy 38 has been shown to significantly remedy powder-induced defects with powder that does not fully comply with the abovementioned requirements, yielding parts with a relative density that was comparable to those processed from higher quality powders 39. It is important to consider the chemical composition of an alloy to be used in SLM since some chemical elements can make an alloy susceptible to cracking, as is common in difficult-to-weld alloys, such as Al-7075. Altering the chemical composition by adding elements that hinder cracking has been demonstrated to improve the process-ability, such as when amounts of Si were added to the Al-7075 to improve the fluidity, therefore eliminating the cracks 46.
The consolidation of continuous single tracks can be used to determine a suitable range for laser power and scan speed for low porosity manufacture, as well as to define the layer thickness and hatch spacing through examination of the melt pool shape 68. The basic requirements of single tracks can be found in 26, 65. The stability of the melt pool is controlled by the processing parameters 25, 54. The laser power and speed affect the width and depth of a scan track (Figure 2b), whereas its length is governed by the laser power and material’s absorptivity 62. Defects, such as satellites, balling, irregularities, and discontinuities 26, can arise in Al tracks when the laser scan speed increases beyond a critical limit. Slower speeds are favoured because they increase the melt volume and enhance
38. However, narrow hatch spacing results in slower rates of production, whilst larger hatch spacing impose a limitation on the maximum layer thickness 70. Increasing the layer thickness promotes the formation of defects in tracks and layers 26, hindering the deposition of uniform layers to build a multi-layered part. Furthermore, a large layer thickness results in reducing the re-melted depth 26.
Two types of pores form during Al SLM, namely metallurgical and
keyhole pores. The type of pore is scan speed dependent. A critical scan speed can be defined 38, below which metallurgical (spherical) pores form and above which keyhole (irregular) pores are created. Altering the scan strategy has been
employed with the aim of controlling the microstructure, minimizing the residual stresses 43, 71, and remedying defects, such as porosity 38.
The metallurgy of SLM Al alloys
A series of thermal processes during SLM 12 affect the resulting
towards the moving heat source. Fast solidification also resulted in a fine and quite homogeneous dispersion of the alloying elements 48 (Figure 3e and f). Prashanth et al. 74 provided a clear explanation of the solidification process in SLM of Al-Si alloys attributing the formation of the cellular structure to the amount of undercooling. During solidification, Si is rejected into the liquid increasing the solute concentration. As per the Al-Si phase diagram, the solubility of Si in Al is reduced at lower temperatures but it can be extended by fast cooling. Therefore, the amount of Si rejected in the liquid during rapid cooling is reduced decreasing the solute concentration in the liquid as well as the undercooling. Rapid solidification changes the solute distribution drastically 75. Thus a cellular structure is favoured in which α-Al solidifies first in a cellular morphology leaving the remaining Si as segregations at the boundaries.
MP core MP boundary
Melt pool core Melt pool boundary
Figure 2: The microstructure of SLM AlSi10Mg showing (a) the three regions of microstructure within
the melt pools divided into fine grains, coarse grains, and heat affected zones HAZ 43, (b) equiaxed
grains observed on the plane perpendicular to the build direction with coarser grains at the melt pool
boundary, and (c) fine equiaxed grains at the melt pool core and coarser elongated grains at the melt
pool boundary as seen in the plane parallel to the build direction 48. (d) SEM image demonstrating a
similar microstructure achieved for AlSi12 using SLM with (e and f) EDX maps showing the good
dispersion of the alloying elements 74.
During solidification, a fraction of the grains grow faster in preferred orientations, i.e. formation of a crystallographic texture develops in the material 43 due to the directional solidification and layer-by-layer fabrication (Figure 4a). Thijs et al. 43 reported the crystallographic texture of AlSi10Mg to change from a strong fibre texture to a weak cubic texture by changing the scan strategy (Figure 4b).
Figure 3: (a) EBSD orientation maps for SLM AlSi10Mg samples processed using the meander scan
strategy and (b) the effect of changing the scan strategy on the crystallographic texture of the SLM
AlSi10Mg material 43.
The response of SLM Al to various post-manufacture heat treatments has been investigated in the literature. Annealing SLM Al-20%Si 76, Al-12%Si 74, and AlSi10Mg 50, 77 led to Si diffusion to form particles (Figure 5a). As the treatment temperature or duration increased, the microstructure coarsened 74. Heat treating AlSi10Mg 20, 48 and 7075 46 using solution heat treatment followed by artificial ageing (T6) also returned the same phase transformation (Figure 5b),
spherodisation (Figure 5c). Both heat treatment procedures dissolved the melt pools and dendritic structure. As the treatment duration increased, Si had a longer duration to diffuse and formed larger particles, decreasing their spatial density and increasing their size 48.
Figure 4: The microstructure of SLM AlSi10Mg after annealing heat treatment (a) 50 and solution heat
treatment followed by artificial ageing (b) 48. Both heat treatments promoted spherodisation phase
transformation as illustrated in (c) 74.
The mechanical performance of SLM Al alloys
Material-laser interaction and rapid solidification due to high cooling rates (~ 105 K/s 60) lead to microstructural modifications that can yield enhanced material properties 36 compared to CM material, e.g. cast material 45. Mechanical characterization to assess the feasibility of using SLM for structural parts is ongoing, as demonstrated by the examples in Table II. Also, a summary of the tensile mechanical properties of SLM Al alloys reported in the literature can be found in 37. Generally, SLM parts are characterized by high residual stresses arising from high energy density and rapid solidification 78. High residual stresses in SLM AlSi12 (~36 MPa) were reduced by almost 90% by using a heated-build plate and post-process stress relief treatment 79. The microstructure and porosity controlled by the process parameters influence the mechanical behaviour 20. The
fine microstructure and good distribution of alloying elements (at the scale of several tens of microns) in SLM yield uniform local mechanical properties across the melt pools 49. The global mechanical properties of SLM materials are
comparable to those of their conventionally processed counterparts. Mechanical anisotropy is affected by the material’s crystallographic texture 80, 81, which is attributed to the process parameters 43, 80. The layer-by-layer fashion in which the parts are built in SLM results in a number of factors leading to anisotropy 82. These are: (1) the shape and size of voids, (2) the grain orientation and
crystallographic texture with respect to the build orientation, and (3) the regions of interface between scan tracks and layers. When anisotropy is observed, better properties are generally seen along axes perpendicular to the BD 20, 22, 80, with the density of dislocations being dependent on the BD 81. However in some cases, no significant BD effect was observed 20, 45.
Table II: A list of the studies in the literature that investigated the various mechanical
properties of SLM Al alloys.
AlSi10Mg AlSi12 AlSi50 A357 Al-7075
Nano-hardness 26, 47, 49, 73
Micro-hardness 22, 48, 80, 83 57 46 83
22, 45, 49, 52, 77, 80, 84
42, 74, 79,
85, 86 56 55
Fatigue performance 20, 53, 87, 88 60, 79, 86 55
Fracture toughness 60
Creep resistance 45
Impact resistance 80
Wear behaviour 57, 58
ductility without significantly reducing strength, providing a good compromise for applications which require both properties. The compromise between the SLM material’s strength and ductility that can be achieved via heat treatment is
appealing for numerous applications when considering the material’s
comparatively low density. A T6 heat treatment has been shown to soften SLM AlSi10Mg 48 and 7075 46. The strengthening factors in the as-built and heat-treated materials were similar except for the grain size refinement factor in the former being replaced by the strengthening effect of dispersoids (Orowan) in the latter. The higher hardness in the SLM material indicates that the grain size refinement effect outweighed the dispersoid effect in this case.
The presence of un-bonded powder inside SLM parts was reported for AlSi10Mg 38, 45, 6061 44, and 7075 55. Although these regions are relatively small, i.e. they will not significantly reduce the load bearing area under tension 45, they might be influential to fatigue. Defects in SLM parts act as stress concentrations, depressing fatigue life due to crack nucleation and growth 20, 78, 89-91. SLM Al has shown good performance under cyclic loading 20, 53. The potential effect of
machining to improve the fatigue performance was emphasised in some studies in the literature 12, however, Aboulkhair et al. 53 provided evidence that machining may not improve the fatigue performance but rather increases the scatter in lifetime data. Heat treatment has been shown to considerably improve the fatigue performance 20, 53 due to the transformation of Si dendrites to spheroids that hinder crack initiation and propagation 20, 53. The optimum fatigue life can be achieved by a combination of heat treatment and surface machining. The enhancement in fatigue life via heat treatment was attributed to the induced ductility and relaxation of residual stresses. Failure under tensile and cyclic loading always originated at sub-surface defects and propagated along the melt pool boundaries, this being the weaker region since it is Al-rich.
sector. This section will highlight some of these areas, demonstrating their importance.
SLM commonly uses readily available pre-alloyed metal powder. The development of new SLM tailored powder mixtures has strong potential.
Blending metal powders with different properties is a promising route. This could be in the form of altering the composition of pre-alloyed powder through adding modifiers or designing new alloys as in the case of SCALMALLOY® 92. Coating Al or mixing it with elements that would enhance its absorptivity or surface tension could be a means for better material process-ability. The laser surface alloying literature 93-95 is rich with examples for improving the laser absorptivity through suitable additives. Depositing Cu on Al particles yielded particles with intermediate absorptivity and reflectance compared to the original elements 96. Sistiaga et al. 46 added Si to Al-7075 alloy to improve the fluidity of the alloy, reduce the thermal expansion, and decrease the solidification range; successfully hindering the cracking common in SLM of Al-7075, producing defect-free parts. Vora et al. 97 compared processing pre-alloyed AlSi12 powder to blended Al and Si powder to the same composition demonstrating lower residual stressed when using blended powders. A means for mixing powders without just blending is satelliting 98, 99 which is yet to be applied in SLM. Despite the potential in this approach, it is worth investigating the practicality of recycling the blended powders.
Several studies have stated the importance of using metal powders that have properties suitable for SLM. Standardizing properties of powders to be used for SLM is essential to cope with the process needs through producing powder with specifications meeting the process requirements. One of the appealing features in SLM is the ability to recycle the leftover powder. However, the literature on Al alloys lacks information on the threshold limit for powder recycling after which the quality of the produced parts and their mechanical performance is compromised. There are several studies on the powder recycling for other metal powders used in SLM 100, 101 but the findings cannot be
over powder that has been found to have different properties from an alloy to another 64. For example, the laser spatter from Ti-6Al-4V is not significantly different from the fresh powder, unlike AlSi10Mg spatter which has a distinct morphology and chemical composition.
As has been demonstrated in Table I, most of the research to date has been with Al-Si casting alloys with less consideration of the high strength alloys. This is due to the relative ease of processing the former compared to the latter, which in most cases not easily weldable, which is also indicative that they are not easily processed by SLM. The success of processing a hard-to-process alloy, such as Al-7075, through changing the chemical composition introduces the promising approach that is logical to adopt to widen the range of focus of aluminium alloys used in SLM. In addition to changing the chemical composition of alloys for better process-ability, chemical elements can be mixed into Al alloys with the aim
of in-situ production of reinforced Al-based composites 102, 103, such as AlSi10Mg
and SiC with multiple reinforcements yielding superior mechanical properties 104, 105, TiC reinforced Al-Si-Mg nano-composite from a mechanically-alloyed AlSi10Mg and TiC 106, and TiC reinforced composite from mechanically-alloyed titanium, aluminium, and graphite 107.
1. M. Baumers, C. Tuck, R. Wildman, I. Ashcroft, E. Rosamond, R. Hague, 23rd Solid Freeform Fabr. Symp.(The University of Texas at Austin, Austin, TX, 2012), pp.932.
2. M. Baumers, C. Tuck, R. Wildman, I. Ashcroft, E. Rosamond, R. Hague, , J. Ind. Ecol. 17, 418 (2013).
3. B. Zhang, H. Liao, C. Coddet, Mater. Des. 34, 753 (2012).
4. B. Ferrar, L. Mullen, E. Jones, R. Stamp, C.J. Sutcliffe, J. Mater. Process. Tech.
212(2), 355 (2012).
5. I. Yadroitsev, P. Bertrand, I. Smurov, Appl. Surf. Sci. 253(19), 8064 (2007). 6. R. Li, Y. Shi, Z. Wang, L. Wang, J. Liu, W. Jiang, Appl. Surf. Sci. 256(13)
7. M. Baumers, C. Tuck, R. Wildman, I. Ashcroft, R. Hague, J. Ind. Ecol. (2016), in press.
8. I. Gibson, D.W. Rosen, B. Stucker, Additive Manufacturing Technologies, Springer (2010).
9. L. Loeber, S. Biamino, U. Ackelid, S. Sabbadini, P. Epicoco, P. Fino, J. Eckert, 22nd Solid Freeform Fabr. Symp.(The University of Texas at Austin, Austin, TX, 2011), pp. 547.
10. K. Kempen, B. Vrancken, L. Thijs, S. Buls, J. Van Humbeeck, J.-P. Kruth, SFF 24, (2013).
11. D. Buchbinder, W. Meiners, N. Pirch, K. Wissenbach, J. Schrage, J. Laser Appl. 26(1), 012004 (2014).
12. W.E. Frazier, J. Mater. Eng. Perform. 23(6), 12 (2014).
13. B.D. L., R.D. W., L. Ming, 3D Print. Addit. Manuf. 1(1), 4 (2014).
14. V. Matilainen, H. Piili, A. Salminen, T. Syvänen, O. Nyrhilä, Phys. Procedia
56(0), 317 (2014).
15. D.L. Bourell, J. Joseph J Beaman, M.C. Leu, D.W. Rosen, US – TURKEY Workshop On Rapid Technologies (2009).
16. D.C. Hofmann, S. Roberts, R. Otis, J. Kolodziejska, R.P. Dillon, J.O. Suh, A.A. Shapiro, Z.K. Liu, J.P. Borgonia, Sci. Rep. 4, 5357 (2014).
17. N. Guo, M.C. Leu, Front.Mech. Eng. 8(3) 215 (2013).
18. S. Leuders, M. Thöne, A. Riemer, T. Niendorf, T. Tröster, H.A. Richard, H.J. Maier, Int. J. Fatigue 48(0), 300 (2013).
19. H. Schleifenbaum, W. Meiners, K. Wissenbach, C. Hinke, J. Manuf. Sci. Technol. 2(3), 161 (2010).
20. E. Brandl, U. Heckenberger, V. Holzinger, D. Buchbinder, Mater. Des. 34(0), 159 (2012).
21. C.J. Tuck, R.J.M. Hague, M. Ruffo, M. Ransley, P. Adams, Int. J. Comput. Integ. M. 21(3), 245 (2008).
22. D. Buchbinder, H. Schleifenbaum, S. Heidrich, W. Meiners, J. Bültmann, Phys. Procedia 12, Part A(0), 271 (2011).
24. I. Maskery, N.T. Aboulkhair, A.O. Aremu, C.J. Tuck, I.A. Ashcroft, R.D. Wildman, R.J.M. Hague, Mater. Sci. Eng. A 670, 264 (2016).
25. I. Yadroitsev, A. Gusarov, I. Yadroitsava, I. Smurov, J. Mater. Process. Tech.
210(12), 1624 (2010).
26. N.T. Aboulkhair, I. Maskery, C. Tuck, I. Ashcroft, N.M. Everitt, J. Mater. Process. Tech. 230, 88 (2016).
27. N.T. Aboulkhair, Additive manufacture of an aluminium alloy: processing, microstructure, and mechanical properties, Department of Mechanical, Materials, and Manufacturing Engineering, University of Nottingham, UK, 2015.
28. E. Herderick, Proceedings of MS&T 2011 (2011).
29. K.V. Wong, A. Hernandez, ISRN Mech. Eng. 2012, 1 (2012).
30. E.O. Olakanmi, R.F. Cochrane, K.W. Dalgarno, Prog. Mater. Sci. 74(0), 401 (2015).
31. M. Tisza, Physical metallurgy for engineers, ASM International and Fruend Publishing House Ltd.2002.
32. Y. Li, D. Gu, Mater. Des. 63(0), 856 (2014).
33. G.E. Totten, D.S. Mackenzie, Handbook of Aluminum: Physical Metallurgy and Processes, 1 ed., CRC press, New York, 2003.
34. I.J. Polmear, Light alloys: metallurgy of the light metals, 3rd edition ed. 35. W.H. Hosford, Physical Metallurgy, Second ed., CRC Press, United States of America, 2010.
36. S. Dadbakhsh, L. Hao, J. Alloy. Compd. 541(0), 328 (2012).
37. Y. Ding, J.A. Muñiz-Lerma, M. Trask, S. Chou, A. Walker, M. Brochu, MRS Bulletin 41(10),745 (2016).
38. N.T. Aboulkhair, N.M. Everitt, I. Ashcroft, C. Tuck, Addit. Manuf. 1-4(0), 77 (2014).
39. N.T. Aboulkhair, I. Maskery, I. Ashcroft, C. Tuck, N.M. Everitt, Lasers in Manufacturing conference, (Munich, Germany, 2015).
41. Handbook of Aluminum: Volume 2: Alloy Production and Materials Manufacturing, 2003.
42. X.J. Wang, L.C. Zhang, M.H. Fang, T.B. Sercombe, Mater. Sci. Eng.A
597(0), 370 (2014).
43. L. Thijs, K. Kempen, J.-P. Kruth, J. Van Humbeeck, Acta Mater. 61(5), 1809 (2013).
44. E. Louvis, P. Fox, C.J. Sutcliffe, J. Mater. Process. Technol. 211(2), 275 (2011).
45. N. Read, W. Wang, K. Essa, M.M. Attallah, Mater. Des. 65(0), 417 (2015). 46. M.L. Montero Sistiaga, R. Mertens, B. Vrancken, X. Wang, B. Van
Hooreweder, J.-P. Kruth, J. Van Humbeeck, J. Mater. Process. Technol. 238, 437 (2016).
47. N.T. Aboulkhair, I. Maskery, C. Tuck, I. Ashcroft, N. Everitt, SPIE, 2015, pp. 965702-965702-7.
48. N.T. Aboulkhair, C. Tuck, I. Ashcroft, I. Maskery, N.M. Everitt, Metall. Mater. Trans. A 46A(8), 3337 (2015).
49. N.T. Aboulkhair, I. Maskery, C. Tuck, I. Ashcroft, N.M. Everitt, Mater. Sci. Eng. A 667, 139 (2016).
50. I. Maskery, N.T. Aboulkhair, M.R. Corfield, C. Tuck, A.T. Clare, R.K. Leach, R.D. Wildman, I.A. Ashcroft, R.J.M. Hague, Mater. Charact. 111, 193 (2016). 51. J. Wu, X.Q. Wang, W. Wang, M.M. Attallah, M.H. Loretto, Acta Mater. 117, 311 (2016).
52. I. Rosenthal, A. Stern, N. Frage, Metallography, Microstructure, and Analysis
3(6), 448 (2014).
53. N.T. Aboulkhair, I. Maskery, C. Tuck, I. Ashcroft, N.M. Everitt, Mater. Des.
104, 174 (2016).
54. B. Ahuja, M. Karg, K.Y. Nagulin, M. Schmidt, Phys. Procedia 56(0), 135 (2014).
55. W. Reschetnik, J.P. Brüggemann, M.E. Aydinöz, O. Grydin, K.P. Hoyer, G. Kullmer, H.A. Richard, Procedia Structural Integrity 2, 3040 (2016).
57. N. Kang, P. Coddet, C. Chen, Y. Wang, H. Liao, C. Coddet, Mater. Des. 99, 120 (2016).
58. N. Kang, P. Coddet, H. Liao, T. Baur, C. Coddet, Appl. Surf. Sci. 378, 142 (2016).
59. X.P. Li, K.M. O’Donnell, T.B. Sercombe, Addit. Manuf. 10, 10 (2016). 60. J. Suryawanshi, K.G. Prashanth, S. Scudino, J. Eckert, O. Prakash, U. Ramamurty, Acta Mater. 115, 285 (2016).
61. P. Ma, Y. Jia, K.G. Prashanth, S. Scudino, Z. Yu, J. Eckert, J. Alloy. Compd.
657, 430 (2016).
62. C. Kamath, B. El-dasher, G.F. Gallegos, W.E. King, A. Sisto, Livermore, California. UNT Digital Library.
http://digital.library.unt.edu/ark:/67531/metadc872227/. Accessed October 26, 2016.
63. C. Tuck, I. Maskery, M. Simonelli, N. Aboulkhair, I. Ashcroft, N. Everitt, R. Wildman, R. Hague, TMS Annual meeting and exhibition, 2015.
64. M. Simonelli, C. Tuck, N.T. Aboulkhair, I. Maskery, I. Ashcroft, R.D. Wildman, R. Hague, Metall. Mater. Trans. A 46A(9), 3842 (2015).
65. K. Kempen, L. Thijs, E. Yasa, M. Badrossamay, W. Verheecke, J.-P. Kruth, 22nd Solid Freeform Fabr. Symp. (The University of Texas at Austin, Austin, TX, 2011), pp. 484-495.
66. D. Dai, D. Gu, Mater. Des. 55(0), 482 (2014).
67. I. Yadroitsev, P. Krakhmalev, I. Yadroitsava, S. Johansson, I. Smurov, J. Mater. Process. Technol. 213(4), 606 (2013).
68. Y. Pupo, J. Delgado, L. Serenó, J. Ciurana, Procedia Eng. 63(0), 370 (2013). 69. W.E. King, H.D. Barth, V.M. Castillo, G.F. Gallegos, J.W. Gibbs, D.E. Hahn, C. Kamath, A.M. Rubenchik, J. Mater. Process. Technol. 214(12), 2915 (2014). 70. X. Su, Y. Yang, J. Mater. Process. Technol. 212(10), 2074 (2012).
73. Nicola M. Everitt, Nesma T. Aboulkhair, Ian Maskery, Chris Tuck, I. Ashcroft, Adv. Mater. Letters 7(1), 13 (2016).
74. K.G. Prashanth, S. Scudino, H.J. Klauss, K.B. Surreddi, L. Löber, Z. Wang, A.K. Chaubey, U. Kühn, J. Eckert, Mater. Sci. Eng. A 590(0), 153 (2014). 75. W. Kurz, R. Trivedi, Metall. Mater. Trans. A22(12), 3051 (1991).
76. P. Ma, K.G. Prashanth, S. Scudino, Y.D. Jia, H.W. Wang, C.M. Zou, Z.J. Wei, J. Eckert, Metals 4(1), 28 (2014).
77. W. Li, S. Li, J. Liu, A. Zhang, Y. Zhou, Q. Wei, C. Yan, Y. Shi, Mater. Sci. Eng. A 663, 116 (2016).
78. P. Edwards, M. Ramulu, Mater. Sci. Eng. A 598(0), 327 (2014).
79. S. Siddique, M. Imran, E. Wycisk, C. Emmelmann, F. Walther, , J. Mater. Process. Technol. 221(0), 205 (2015).
80. K. Kempen, L. Thijs, J. Van Humbeeck, J.P. Kruth, Phys. Procedia 39(0), 439 (2012).
81. P. Kanagarajah, F. Brenne, T. Niendorf, H.J. Maier, Mater. Sci. Eng. A
588(0), 188 (2013).
82. D. Buchbinder, W.Meiners, K. Wissenbach, R. Poprawe, J. Laser Appl. 27, S29205 (2015).
83. K. Bartkowiak, S. Ullrich, T. Frick, M. Schmidt, Phys. Procedia 12, Part A(0), 393 (2011).
84. U. Tradowsky, J. White, R.M. Ward, N. Read, W. Reimers, M.M. Attallah, Mater. Des. 105, 212 (2016.
85. K.G. Prashanth, R. Damodaram, S. Scudino, Z. Wang, K. Prasad Rao, J. Eckert, Mater. Des. 57(0), 632 (2014).
86. S. Siddique, M. Imran, F. Walther, Int. J. Fatigue, in press.
87. I. Maskery, N.T. Aboulkhair, C. Tuck, R.D. Wildman, I.A. Ashcroft, N.M. Everitt, R.J.M. Hague, 26th Solid Freeform Fabr. Symp. (The University of Texas at Austin, Austin, TX, 2015), pp. 1017-1025.
88. M. Tang, P. Chris Pistorius, Int. J. Fatigue, in press.
90. Eliahu Zahavi, V. Torbilo, Fatigue design - Life expectancy of machine parts, CRC Press 1996.
91. S. Suresh, Fatigue of materials, 2nd ed., Cambridge University Press 1998. 92. Airbus-Group, SCALMALLOY®RP Auminum-Magnesium-Scandium alloy powder.
<http://www.technology-licensing.com/etl/int/en/What-we- offer/Technologies-for-licensing/Metallics-and-related-manufacturing-technologies/Scalmalloy-RP.html>, (accessed 19 Novermber 2014.2014). 93. R.S. Razavi, G.R. Gordani, Laser Surface Treatments of Aluminum Alloys, in: P.Z. Ahmed (Ed.), Recent Trends in Processing and Degradation of
Aluminium Alloys, InTech, 2011.
94. D.S. Gnanamuthu, Laser Surface Treatment, Optic. Eng. 19(5), 195783 (1980).
95. S. Tomida, K. Nakata, S. Saji, T. Kubo, Surf. Coat. Technol. 142–144, 585 (2001).
96. M. Sachs, O. Hentschel, J. Schmidt, M. Karg, M. Schmidt, K.-E. Wirth, Phys. Procedia 56(0), 125 (2014).
97. P. Vora, K. Mumtaz, I. Todd, N. Hopkinson, Addit. Manuf. 7, 12 (2015). 98. A. Clare, A. Kennedy, Additive manufacturing, Patent number US 20160279703 A1,The University of Nottingham, United Kingdom, 2016. 99. A.N.D. Gasper, S. Catchpole-Smith, A.T. Clare, J. Mater. Process. Technol.
239, 230 (2017).
100. L.C. Ardila, F. Garciandia, J.B. González-Díaz, P. Álvarez, A. Echeverria, M.M. Petite, R. Deffley, J. Ochoa, Phys. Procedia 56(0), 99 (2014).
101. V. Seyda, N. Kaufmann, C. Emmelmann, Phys. Procedia 39, 425 (2012). 102. S. Dadbakhsh, L. Hao, The Scientific World Journal 2014, 106129 (2014). 103. S. Dadbakhsh, L. Hao, P.G.E. Jerrard, D.Z. Zhang, Powder Technol. 231(0), 112 (2012).
106. D.D. Gu, H.Q. Wang, D.H. Dai, P.P. Yuan, W. Meiners, R. Poprawe, Scripta Mater. 96(0), 25 (2015).
107. D. Gu, Z. Wang, Y. Shen, Q. Li, Y. Li, Appl. Surf. Sci. 255(22), 9230 (2009).
Nesma T. Aboulkhair
Additive Manufacturing and 3D Printing Research Group Faculty of Engineering, University of Nottingham
Nottingham, NG7 2RD, United Kingdom.
Nesma is a research fellow in the centre for AM. She holds a BSc in Mechanical Engineering from Cairo University, MSc in Mechanical Engineering from the American University in Cairo, and PhD in Materials Engineering and Materials Design from the University of Nottingham. Nesma was awarded numerous fellowships and prizes throughout her studies. Her current research spans across various AM processes. She has a broad experience in metal additive manufacturing and strong knowledge in metallurgy and materials characterisation.
Nicola M. Everitt
Bioengineering Research Group
Faculty of Engineering, University of Nottingham Nottingham, NG7 2RD, United Kingdom.
Dr. Nicola Everitt (B.Sc. (Hons) in Materials Science and D.Phil. (Oxon)) has been an Associate Professor at the University of Nottingham in the
Additive Manufacturing and 3D Printing Research Group Faculty of Engineering, University of Nottingham
Nottingham, NG7 2RD, United Kingdom.
Ian Maskery attended the University of York for four years until 2009, obtaining an MPhys degree with first class honours. He obtained his PhD in Physics from the University of Warwick in 2013. Since then, Ian has been a postdoctoral researcher at the University of Nottingham, where he has
investigated the properties of materials made by selective laser melting. Ian also investigates the use of lightweight cellular structures in additive manufacturing, examining relationships between their design, manufacture and mechanical performance.
Additive Manufacturing and 3D Printing Research Group Faculty of Engineering, University of Nottingham
Nottingham, NG7 2RD, United Kingdom.
Ian Ashcroft is Professor of Solid Mechanics at the University of
Nottingham. His expertise is in both experimental and computational mechanics with particular interest in the effects of complex loading and environment on materials and structures. Recently, he has focussed his research into the application of solid mechanics to additive manufacturing, particularly in developing multi-physics modelling techniques for AM processes and the post processing performance of parts and the development of design and optimisation techniques for various AM technologies.
Nottingham, NG7 2RD, United Kingdom.